Alloys & Their Phase Diagrams Alloys & Their Phase Diagrams
46

# Alloys Steel

Apr 28, 2015

## Documents

11oxendi664

phase diagram for steel
Welcome message from author
Transcript

Alloys & Their Phase DiagramsAlloys & Their Phase Diagrams

Objectives of the classObjectives of the class

Gibbs phase ruleIntroduction to phase diagram

Practice phase diagramLever rule

Important Observation: One question in the midterm

Gibbs phase ruleGibbs phase rule

P + F = C +2

P: number of phases (ie, solid, liquid, or gas)C: number of components

F: Degree of freedom

Simple ExampleSimple ExampleWater:

a) At the triple point:P = 3 (solid, liquid, and gas)

C= 1 (water)P + F = C + 2

F = 0 (no degree of freedom)

b) liquid-solid curveP = 2

2+F = 1 + 2F= 1

One variable (T or P) can be changed

c) LiquidP =1

So F =2Two variables (T and P) can be varied independently

and the system will remains a single phase

Unlimited SolutibityUnlimited Solutibity

Limited solubilityLimited solubility

No SolubilityNo Solubility

Binary Isomorphous Alloy SystemsBinary Isomorphous Alloy Systems

A mixture of two metals is called a binary alloy and constitutes a two-component system.

Each metallic element in an alloy is called a separate component.

Isomorphous systems contain metals which are completely soluble in each other and have a single type of crystal structure.

Cu-Ni: A Substitutional Solid SolutionCu-Ni: A Substitutional Solid Solution

Cu-Ni: Binary Isomorphous Alloy ExampleCu-Ni: Binary Isomorphous Alloy Example

Liquidus line

Solidus line

Tie line

The Lever RuleThe Lever Rule

Fraction of the solid phase = (Wo – Wl)/(Ws-Wl)

To compute the amount of solid phase:

Cu-Ni: Cooling CurvesCu-Ni: Cooling Curves

Cooling curveCooling curve

Some examplesSome examples

Binary Eutectic Alloy SystemsBinary Eutectic Alloy Systems

Eutectic composition:Eutectic composition:

Composition of the phases:Alpha: 19.2% SnBeta: 97.5% Sn

Phases: alpha and beta

Amount of phases:45.5% of alpha: (97.5-61.9)/(97.5-19.2)

54.5% of beta phase

Example: Point DExample: Point D

Composition of the phases:Alpha: 19.2% SnLiquid: 61.9% Sn

Phases: liquid and alpha

Amount of phases:51% of alpha phase: (61.9-40)/(61.9-19.2)

49% of liquid phase

Example: Point EExample: Point E

Composition of the phases:Alpha: 19.2% Snbeta: 97.5% Sn

Phases: alpha and beta

Amount of phases:73% of alpha phase: (97.5-40)/(97.5-19.2)

27% of beta phase

So what? So what?

Soft: eutectic (free flowing): electronic assembyEutetic: from the Greek

easy melting

Plumbers’ solder: pasty used in joints (Romans) and car body fillingHigh-meltingsolder

A Eutectic Cooling CurveA Eutectic Cooling Curve

Temperature-time cooling curvefor 60% Pb – 40% Sn alloy

Eutectic MicrostructuresEutectic Microstructures

There are a number of different “morphologies#” for the two phases in a binary eutectic alloy.

Of prime importance is the minimization of the interfacial area between the phases.

The rate of cooling can also have an important effect.

Eutectic MicrostructuresEutectic MicrostructuresSchematic illustration of the

various eutectic microstructures: (a) lamellar, (b) rodlike, (c) globular, and (d) acicular (or needlelike).

Morphology means the “form”, “shape” or “outward microstructure” of a phase.

Microstructure evolutionMicrostructure evolution

Equilibrium Microstructure of Steel AlloysEquilibrium Microstructure of Steel Alloys

The Iron-Iron Carbide Phase DiagramThe Iron-Iron Carbide Phase Diagram

ferriteBCC iron crystal lattice

AusteniteFCC crystal

CementiteHard and brittle

Steels and IronsSteels and Irons

ForgingForging

ForgingForging

Plain-Carbon SteelPlain-Carbon Steel

Steel can be defined as an Iron alloy which transforms to Austenite on heating.

A plain-carbon steels has no other major alloying element beside carbon.

When a plain-carbon steel is slowly cooled from the Austenitic range it undergoes the eutectoid transformation.

Construction steelConstruction steel

Construction steel alloys used for concrete reinforcing bars and structural shapes have been traditionally been 0.1-0.2% C plain-carbon steels with only minor additional elements.

In general these alloys are called Low-alloy Steel and for most purposes they can be considered plain-carbon steel.

The Iron-Iron Carbide Eutectoid SystemThe Iron-Iron Carbide Eutectoid System

Note: pearlite is not a phase, but a combination of ferrite and cementite

EutectoidEutectoid

Eutectoid MicrostructuresEutectoid MicrostructuresJust like the eutectic systems there are a number of different

“morphologies#” for the two phases in a binary eutectic alloy.

The most common morphology for eutectoid areas in the Fe-Fe3C system is lamellar. (This is because most steel is relatively slowly cooled through the eutectoid phase transformation.)

Evolution of Eutectoid Steel MicrostructureEvolution of Eutectoid Steel Microstructure

Hypoeutectoid Hypereutectoid

Slow Cooling of Plain-Carbon SteelsSlow Cooling of Plain-Carbon SteelsTransformation of a 0.4% C hypoeutectoid plain-carbon

steel with slow cooling.

HypoeutectoidHypoeutectoid

Slow Cooling of Plain-Carbon SteelsSlow Cooling of Plain-Carbon SteelsTransformation of a 1.2% C hypereutectoid plain-carbon steel

with slow cooling.

HypereutectoidHypereutectoid

Carbon Steel (90% of the steel production)Carbon Steel (90% of the steel production)

Low alloy steel (up to 6% of chromium, nickel, etc)

Stainless steel (18% chromium and 8% nickel)

Tool steels ( heavy alloyed with chromium, molybdenum, tungsten, vanadium, and cobalt).

ProblemProblemA 0.45%C hypoeutectoid plain-carbon steel is slowly

cooled from 950 C to a temperature just slightly above 723 C. Calculate the weight percent austenite and weight percent proeutectoid ferrite in this steel.

0.45

0.800.02

Austenite = (0.45-0.02)/(0.80-0.02) = 55.1%

Proeutectoid Ferrite =(0.80-0.45)/(0.8-0.02)

= 44.9

A 0.45%C hypoeutectoid plain-carbon steel is slowlycooled from 950 C to a temperature just slightlybelow 723 C.

(a)Calculate the weight percent proeutectoid ferrite in this steel.

(b) Calculate the weight percent eutectoid ferrite and the weight percent eutectoid cementite in this steel.

Proeutectoid Ferrite =(0.80-0.45)/(0.8-0.02)=44.9%

Cementite = (0.45-0.02)/(6.67-0.02) = 6.5%

0.45

0.800.02 Total ferrite = (6.67-0.45)/(6.67-0.02) = 93.5%Eutectoid ferrite =

total ferrite – proeutectoid ferrite= 93.5 – 44.9 = 48.6%

ProblemProblem

A hypoeutectoid steel contains 22.5% eutectoid ferrite. What is the average carbon content?

Total ferrite= proeutectoid ferrite + eutectoid ferrite

(6.67-x)/(6.67-0.02) = (0.80 –x)/(0.8-0.02) + 0.225

X =0.2

Jominy Hardenability TestJominy Hardenability Test

Intermediate Phases - Cu-Zn ExampleIntermediate Phases - Cu-Zn Example

Hypoeutectoid Phase DiagramHypoeutectoid Phase Diagram

If a steel with a composition x% carbon is cooled from the Austenite region at about 770 °C ferrite begins to form. This is called proeutectoid (or pre-eutectoid) ferrite since it forms before the eutectoid temperature.